Perspective System Chemistry in Catalysis: Facing the Next Challenges in Production of Energy Vectors and Environmental Remediation
Ivano Alessandri 1,2,3,* and Irene Vassalini 1,2,3,*
1 Consorzio Interuniversitario per la Scienza e Tecnologia dei Materiali (INSTM—UdR), Brescia, via Branze 38, 25123 Brescia, Italy 2 Istituto Nazionale di Ottica—Consiglio Nazionale delle Ricerche (INO—CNR), via Branze 38, 25123 Brescia, Italy 3 Department of Information Engineering, University of Brescia, via Branze 38, 25123 Brescia, Italy * Correspondence: [email protected] (I.A.); [email protected] (I.V.); Tel.: +39-0303715475 (I.A.); +39-0303715667 (I.V.)
Abstract: Most of the catalytic processes that assist the production of either renewable energy vectors or degradation of environmental pollutants rely on the interplay among different factors that can be purposely regulated, in order to improve the overall efﬁciency of reactions. This perspective analyzes some recent examples of ‘systemic catalysts’, which are based on the modiﬁcation of the reaction microenvironment and exploitation of concurrent/parasitic reactions or different types of chemical looping, in order to bypass some drawbacks that cannot be easily circumvented by standard approaches. Innovative extensions of those concepts and strategies might inspire new breakthroughs in a variety of key catalytic cycles characterized by high complexity.
Keywords: system chemistry; smart catalysts; CO2RR; OER; environmental pollutants
Citation: Alessandri, I.; Vassalini, I. System Chemistry in Catalysis: 1. Introduction Facing the Next Challenges in System chemistry investigates non-equilibrium systems that are based on homeostatic Production of Energy Vectors and interactions among different species and require a continuous input of energy to operate [1,2]. Environmental Remediation. Complex and dissipative systems are hallmarks of biology and, in general, life sci- Catalysts 2021, 11, 64. ence [3–5]. On the other hand, most of the research activity tends more generally towards https://doi.org/10.3390/ reductionistic approaches, which are often necessary to investigate speciﬁc processes or catal11010064 phenomena. However, most of the real systems are inherently complex. In addition to pharmacology, biochemistry and fundamental research on the origin of life, which are Received: 6 December 2020 all directly linked to the world of biology, several ﬁelds of environmental (including at- Accepted: 1 January 2021 mospheric chemistry and precision agriculture) and computational chemistry, as well as Published: 5 January 2021 materials science, are striving to cope with such a complexity. For example, over the last
Publisher’s Note: MDPI stays neu- few years a few systems of technological interest have been developed by exploiting auto- tral with regard to jurisdictional clai- catalytic processes, such as oscillating reactions. They have been focused on the creation of ms in published maps and institutio- self-sustained actuators [6–8], touch sensors , or paper-based devices for the temporary nal afﬁliations. storage of self-expiring graphical information . From a more fundamental viewpoint, autocatalytic surface reductions have been investigated to tune the growth of metallic nanoparticles , while bistable reactions have been exploited to control gold nanoparticle formation and self-assembly . Copyright: © 2021 by the authors. Li- In the context of catalysis, the study of redox and photoredox catalysts, which takes censee MDPI, Basel, Switzerland. advantage of coupling between different redox cycles, is another ﬁeld in rapid expansion. This article is an open access article In particular, the so called “synergistic catalysis”, which exploits the combined action of distributed under the terms and con- two catalysts and two catalytic cycles to generate new chemical bonds, is an impressive ditions of the Creative Commons At- demonstration of systemic catalysis [13,14]. tribution (CC BY) license (https:// Recently, the translation of system chemistry principles applied to catalysts operating creativecommons.org/licenses/by/ at the solid state over a macroscale was reported by Prins and co-workers . This work 4.0/).
Catalysts 2021, 11, 64. https://doi.org/10.3390/catal11010064 https://www.mdpi.com/journal/catalysts Catalysts 2021, 11, 64 2 of 18
demonstrates the promotion of the catalytic activity of gold nanoparticles through the exploitation of kinetic asymmetry in the energy consumption generated by light irradiation of a photoresponsive hydrogel. Although heterogenous catalysis could represent another natural playground to apply some of the key concepts and strategies that result from a global analysis of complex systems, this approach is still quite underdeveloped. This perspective will brieﬂy analyze, from a system chemistry viewpoint, some of the processes that are currently intensively explored for producing renewable energy vectors or chemicals and destroy/transform environmental pollutants. We will try to highlight the key reaction dynamics in which a catalyst is requested to operate according to smart and adaptive criteria. Non-exhaustive examples of materials and strategies taken from recent literature— most of the papers have been published between 2017 and 2020—as well as future chal- lenges in catalyst’s design will be discussed.
2. Systemic Catalysts: Design Strategies and Selected Examples 2.1. Dynamics of Factors that Inﬂuence the Performances of a Catalyst Temperature ﬂuctuations, availability of reactants, poisoning of active sites, concurrent side reactions, structural and microstructural modiﬁcation are among the main factors that inﬂuence the catalyst’s performances. In many real cases, these parameters undergo signiﬁcant variations during a process, with direct inﬂuence on the rate determining step of a given reaction. For example, in low-temperature combustion (LTC) processes, a major source of instabilities is caused by kinetic and thermokinetic oscillations, originated from a complex interplay among many competitive elementary reactions, which either release and dissipate (e.g., combustion, which is exothermic) or absorb (e.g., pyrolysis, endothermic) heat . Chemical engineering is used to simulate catalytic processes by taking these dynamic modiﬁcations into account. In general, the effects of temperature and pressure/concentration changes can be predicted and mitigated. Moreover, in some notable cases, such as reforming reactions utilized for production of syngas (or combined production of syngas and ethylene, as illustrated in Figure1),
Catalysts 2021concurrent, 11, x FOR PEER REVIEW endo- and exothermic processes are coupled to achieve autothermic3 of conditions, 19
in which the exothermic reaction provides the heat for the endothermic one [17,18].
FigureFigure 1. Example 1. Exampleof oxidative ofcoupling oxidative in autothermal coupling reactions in autothermal for the combined reactions production for of syngas the combined and ethylene production. of See syngas for details. and ethylene. See  for details.
In parallel, lab-scale tools and new analytical methods based on operando-like spec- However,troscopies in most and of the the synergistic cases,quantitative combination of complementary predictions techniques of variations (see, for in exam- a catalyst’s structure and microstructureple, all-dielectric optical are extremelyantennas for mass challenging. spectrometry For and this Raman/FTIR reason, spectroscopy in-situ character- ization underm operando-likeulti-modal analysis) conditions have been recently is often developed the only in order way to characterize to obtain chemical reliable re- data. In actions in real-world conditions, getting rid of interferences that are usually caused by the use of conventional signal enhancers, such as plasmonic nanoparticles [20–26]. In-situ studies revealed that most of the heterogeneous catalysts evolve their struc- ture and microstructure during the process, so that their original properties are often very different from those observed in working regime [27,28]. In general, a progressive deacti- vation is a common fate for all the catalytic systems, however in many cases the perfor- mance of a catalyst reaches its maximum after several catalytic cycles. Smart “switchable” catalysts, able to respond and adapt to drastic changes of the ex- ternal parameters are going to be developed in many contexts . These types of catalysts are designed to control diffusion dynamics and aggregation states as a function of changes of different stimuli—such as temperature, pH, ionic strength, light, magnetic, and electric fields. However, a systemic approach in catalyst’s design is not limited to the exploitation of these types of external stimuli, but aims at envisioning different scenarios during a cat- alytic reaction, in order to identify the most critical steps and, hopefully, transform limi- tations and drawbacks into advantages. This means that the horizons of several catalytic processes should be broadened through the interconnection/coupling among different and even concurrent reactions. To do that, a preliminary evaluation of all possible reac- tions occurring under working conditions should be carefully carried out. For example, the dry reforming methane reaction,
CH4 + CO2 ⇄ 2 H2 + 2 CO ΔH° = +247 KJ/mol (1) can be accompanied by a number of other concurrent reactions, such as the water–gas shift reaction
CO2 + H2 ⇄ H2O + CO ΔH° = + 41 KJ/mol (2) Other related reforming reactions can occur
Catalysts 2021, 11, 64 3 of 18
this context, a number of characterization techniques based on synchrotron radiation have been gaining ever-growing interest in the last years . In parallel, lab-scale tools and new analytical methods based on operando-like spec- troscopies and the synergistic combination of complementary techniques (see, for example, all-dielectric optical antennas for mass spectrometry and Raman/FTIR spectroscopy multi- modal analysis) have been recently developed in order to characterize chemical reactions in real-world conditions, getting rid of interferences that are usually caused by the use of conventional signal enhancers, such as plasmonic nanoparticles [20–26]. In-situ studies revealed that most of the heterogeneous catalysts evolve their structure and microstructure during the process, so that their original properties are often very differ- ent from those observed in working regime [27,28]. In general, a progressive deactivation is a common fate for all the catalytic systems, however in many cases the performance of a catalyst reaches its maximum after several catalytic cycles. Smart “switchable” catalysts, able to respond and adapt to drastic changes of the external parameters are going to be developed in many contexts . These types of catalysts are designed to control diffusion dynamics and aggregation states as a function of changes of different stimuli—such as temperature, pH, ionic strength, light, magnetic, and electric ﬁelds. However, a systemic approach in catalyst’s design is not limited to the exploitation of these types of external stimuli, but aims at envisioning different scenarios during a catalytic reaction, in order to identify the most critical steps and, hopefully, transform limitations and drawbacks into advantages. This means that the horizons of several catalytic processes should be broadened through the interconnection/coupling among different and even concurrent reactions. To do that, a preliminary evaluation of all possible reactions occurring under working conditions should be carefully carried out. For example, the dry reforming methane reaction,
◦ CH4 + CO2 2 H2 + 2 CO ∆H = +247 KJ/mol (1) can be accompanied by a number of other concurrent reactions, such as the water–gas shift reaction ◦ CO2 + H2 H2O + CO ∆H = + 41 KJ/mol (2) Other related reforming reactions can occur
◦ CH4 + H2O 3 H2 + CO ∆H = +206 KJ/mol (3) ◦ CH4 + 2 H2O 4 H2 + CO2 ∆H = +165 KJ/mol (4) Moreover, coke formation, which is one of the main causes of catalyst’s deacti- vation, is directly inﬂuenced by temperature and pressure conditions. In particular, methane decomposition
◦ CH4 C + 2 H2 ∆H = +75 KJ/mol (5) is an endothermic reaction, i.e., favored at high temperature. On the other hand, CO disproportionation to carbon coke and carbon dioxide
◦ 2 CO C + CO2 ∆H = −172 KJ/mol (6) occurs at low temperature and high pressure. This means that carbon coke can be formed at both high and low temperature. As a result, temperature cannot be exploited as a helpful factor to avoid its formation. However, playing with the equilibrium law of mass, it would be possible to shift Equation (6) towards the formation of CO by adding CO2. At the same time, low temperature and high concentration of CO2 can induce the formation of C coke at low temperature, through the following reactions
◦ CO2 + 2H2 C + 2 H2O ∆H = −90 KJ/mol (7) Catalysts 2021, 11, 64 4 of 18
◦ CO + H2 C + H2O ∆H = −131 KJ/mol (8) This example illustrates the complex systems of chemical reactions that can take place in gas reactions involving small and simple molecules, such as CO2, CH4, CO, O2,H2,H2O, yet analogous arguments can be easily extended to the chemistry of N2, NOx, NH3, SOx, and volatile organic compounds. In general, the design of a catalyst cannot avoid investigating a given process from a systemic viewpoint of complex side reactions. This applies also to electrocatalysis, where different concurrent reactions can occur in the same potential window. One example is given by chlorine evolution, which competes with oxygen evolution in water splitting processes based on salt water . Along the same line, the selectivity and overall efﬁciency of a photocatalytic reaction can be strongly modulated by controlling the parameters that govern a system .
2.2. Selected Examples of Systemic Catalytic Strategies Here we will analyze few examples, taken from recent literature, in which catalytic reactions take advantage of the development of systemic catalysts to improve reaction kinetics and/or selectivity. In particular, in this perspective we will focus our attention on reactions utilized for production of energy vectors and degradation of environmental pollutants. Different general strategies, which are alternative or complementary to static catalytic systems, can be sketched out (Figure2). Figure2a outlines a general process, in which the initial reagents interact to give rise to different intermediates, which eventually evolve in the formation of a targeted compound and, in many cases, other side-products. This reaction ﬂow can be purposely altered by manipulating the catalyst’s local environment at a certain intermediate stage, in order to limit or suppress the formation of byproducts (Figure2b). The manipulation of catalyst’s local environment can be also introduced to directly convert undesired byproducts into product(s) (Figure2c), and several loops can be designed by a synergistic combination of different possible pathways (Figure2d). This Catalysts 2021, 11, x FOR PEER REVIEWscheme represents only a few experimental strategies that can be applied in different5 of 19 real
cases. Many other variations can be introduced and adapted to each speciﬁc process.
FigureFigure 2. Schemes 2. Schem ofe differents of different catalytic catalytic strategies strategies utilized utilized toto promotepromote selectivity selectivity and and yield yield of a of given a given process process:: (a,b) systemic (a,b) systemic approachapproach based based on the on manipulation the manipulation of catalyst’s of catalyst’s local local environment environment for for the the limitation limitation of of byproductsbyproducts formation; (c (c) )sys- systemic temic approach based on the manipulation of local environment for the smart conversion of undesired byproducts into approach based on the manipulation of local environment for the smart conversion of undesired byproducts into targeted targeted products; (d) systemic approach based on design of chemical loops that take advantage of the manipulation of products;the local (d) systemic environment approach at different based stages on designof the process of chemical and might loops leverage that take on concurrent advantage reactions of the. manipulation of the local environment at different stages of the process and might leverage on concurrent reactions. 2.3. Manipulating the Local Microenvironment: The Case of Copper Catalysts for CO2 Reduction and Related Reactions
Electroreduction of carbon dioxide (CO2RR) is one of the most investigated process to transform CO2 into value-added products, including carbon-neutral fuels and a variety of C1 (CO, HCOOH, CH4), C2 (C2H4, CH3COOH, C2H5OH), and C3 (CH3(CH2)2OH) chem- icals. In a recent paper X. Wang, A. Xu et al. (Sargent’s group) succeeded in obtaining me- thane from CO2RR with high selectivity at current densities >100 mA cm−2 and Faraday Efficiency of 48% . This remarkable result has been achieved by controlling the local concentration of CO2 available at the sites of a catalyst made of a 100 nm-thick layer of Cu sputtered on polytetrafluoroethylene (PTFE) membrane. This strategy relied on DFT cal- culations, which revealed that low selectivity in methane production is originated by the free energy barrier in conversion of CO2 into adsorbed carboxylates (*COOH), the first step of a sequence of reactions that lead to the synthesis of methane
∗ ∗ ∗ ∗ CO2 → COOH → CO → CHO → ⋯ → CH4 (9) where the species adsorbed on the Cu catalysts are indicated by an asterisk. The poor selectivity towards methane formation is due to the C–C coupling reaction, which starts with the formation of OCCOH species and leads to the formation of ethylene. This reaction competes with protonation of CO to CHO, which will evolve up to methane synthesis. The authors found out that lowering the coverage of CO2 on the catalyst increases the free energy of COOH*, resulting in lower coverage of CO*. The difference in free energy between CHO and OCCOH shows that a lower coverage of CO* favors methane vs. C2 selectivity. A systematic analysis of the reaction products at different concentration of CO2 (25, 50, 75, 100%) in the reaction gas stream, carried out at different ranges of current den- sity (from 50 to 250 mA cm−2) revealed an optimum in methane selectivity for a gas stream with a CO2 concentration of 75% at 225 mA cm−2. Using a pure (100%) CO2 stream, the
Catalysts 2021, 11, 64 5 of 18
2.3. Manipulating the Local Microenvironment: The Case of Copper Catalysts for CO2 Reduction and Related Reactions
Electroreduction of carbon dioxide (CO2RR) is one of the most investigated process to transform CO2 into value-added products, including carbon-neutral fuels and a variety of C1 (CO, HCOOH, CH4), C2 (C2H4, CH3COOH, C2H5OH), and C3 (CH3(CH2)2OH) chemicals. In a recent paper X. Wang, A. Xu et al. (Sargent’s group) succeeded in obtaining −2 methane from CO2RR with high selectivity at current densities >100 mA cm and Faraday Efﬁciency of 48% . This remarkable result has been achieved by controlling the local concentration of CO2 available at the sites of a catalyst made of a 100 nm-thick layer of Cu sputtered on polytetraﬂuoroethylene (PTFE) membrane. This strategy relied on DFT calculations, which revealed that low selectivity in methane production is originated by the free energy barrier in conversion of CO2 into adsorbed carboxylates (*COOH), the ﬁrst step of a sequence of reactions that lead to the synthesis of methane
∗ ∗ ∗ ∗ CO2 → COOH → CO → CHO → · · · → CH4 (9)
where the species adsorbed on the Cu catalysts are indicated by an asterisk. The poor selectivity towards methane formation is due to the C–C coupling reaction, which starts with the formation of OCCOH species and leads to the formation of ethy- lene. This reaction competes with protonation of CO to CHO, which will evolve up to methane synthesis. The authors found out that lowering the coverage of CO2 on the catalyst increases the free energy of COOH*, resulting in lower coverage of CO*. The difference in free energy between CHO and OCCOH shows that a lower coverage of CO* favors methane vs. C2 selectivity. A systematic analysis of the reaction products at different concentration of CO2 (25, 50, 75, 100%) in the reaction gas stream, carried out at different ranges of current density (from 50 to 250 mA cm−2) revealed an optimum in methane selectivity for a gas −2 stream with a CO2 concentration of 75% at 225 mA cm . Using a pure (100%) CO2 stream, the yield of methane does not exceed 15% in optimal conditions. In parallel, dilute CO2 streams promote hydrogen evolution reaction (HER). Instead of being competitive, this effect is beneﬁcial for production of methane, as the high concentration of H* promotes the protonation of CO* to CHO*. This work represents an example of a rational design of heterogeneous catalysts based on a systemic approach, which analyzes all possible reaction pathways and strongly modi- ﬁes selectivity and yield of products by modifying the catalyst’s local microenvironment (Figure2b), in particular by playing with easily tunable factors, such as the concentration of reagents and current density. In another work, Li et al. demonstrated that the same catalyst (Cu on PTFE mem- branes) can be utilized in CO2RR to produce ethylene with a Faradaic efﬁciency of 72% at a partial current density of 230 mA cm−2, with a full-cell energy efﬁciency of 20% in a neutral medium . Again, the increase of product selectivity and overall efﬁciency was based on the controlled manipulation of local environment. In particular, the authors exploited N-aryl-substituted tetrahydro-4,40-bipyridine molecules to stabilize reaction intermediates. A detailed analysis of the intermediate steps that lead to ethylene formation revealed the crucial role of coordination of CO* on the Cu surface. Experimentally, the maximum Faradaic efﬁciency is achieved for an intermediate ratio between CO adsorbed in ‘atop’ and ‘bridge’ conﬁgurations. The model drawn from computational analyses shows that the water-mediated electron density transfer of the tetrahydro-bipyridine ﬁlm stabilizes the ‘atop’ CO species, which in turns assist the selective formation of ethylene. A large library of tetrahydro-bipyridine was screened, which allowed to synthesize optimized species, on the basis of their electron-donor efﬁciency. When tetrahydro-bipyridine has a too strong electron-donor tendency, the number of atop-bound CO exceeds the optimal concentration, with detrimental effects on Faradaic efﬁciency. Decreased values of Faraday efﬁciency are observed also for poor-electron donor species that do not allow to stabilize a sufﬁcient number of atop-bound CO molecules. Catalysts 2021, 11, 64 6 of 18
The use of accessory molecules to modify intermediate steps of a catalytic reactions is very exciting and could be extended to a variety of processes, introducing the concept of dynamic co-catalyst in heterogeneous reactions. Analogous approaches are quite common in homogeneous catalyst, but less diffuse in heterogeneous systems, in which catalyst and co-catalyst(s) are both in solid state. Another way to control the local concentration of CO species in CO2RR is represented by nanozymes, a class of inorganic nanoparticles that mimic selectivity and turnover rates of natural enzymes. In a recent work O’Mara et al. demonstrated that Ag/Cu core/shell nanoparticles can simulate enzymatic cascade reaction to produce C2 or C3 products through CO2RR, depending on the potential window at which the process is operated . In this case, CO2 diffuses through the porous Cu shell layer toward the Ag core, where it is partially reduced to CO. CO back diffuses through the copper shell layer, where it is adsorbed and converted, via proton-coupled bimolecular reduction, into C2 or C3 products, which are eventually released outside the shell. This strategy enables to channel the sequence of CO2 reduction reactions into a conﬁned space, with CO molecules that are generated inside the catalyst’s core and are forced to stay in close proximity and interact with the copper shell to form new C-C bonds. Analogous approaches have been recently applied in multi-hollow copper catalysts that concentrate the reduction + intermediates and stabilize the formation of Cu species that promote the formation of C2 and C3 products . One of the biggest challenges in Cu-based catalysts is their modiﬁcation during the reaction, which results in signiﬁcant changes in selectivity. Although in situ characterization techniques have been able to monitor the evolution of surface modiﬁcation as a function of time under operando-like conditions, the prevention or control of this transformation is still hard to be achieved [36,37]. In general, most of the strategies utilized to protect the Cu functionality and preserve selectivity are based on protective layers, such as reduced graphene oxide or cationic surfactants . The main disadvantage of using coating layers is the reduction of the number of accessible sites, which is detrimental for the reaction kinetics. An alternative strategy is based on the use of Cu nanoparticles that modify their morphology under bias, improving the formation of C2 and C3 products during operation . However, general solutions are still under investigation. A promising strategy, in the case of reactions and processes that require Cu to be kept in reduced (metallic) state, in order to prevent its oxidation, could be inspired by a seminal work of the Linic’s group on ethylene epoxidation . This reaction is normally affected by surface oxidation of the Cu catalyst, which typically occurs under working condition (T = 400–500 ◦C) and strongly decreases reaction selectivity. This work demonstrated that visible light irradiation (580 nm) can excite localized surface plasmon resonance, leading to the reduction of the freshly formed oxide. This restores the original selectivity and can sustain the reaction under industrial-compatible conditions. Although this approach is indeed quite general and applicable to a variety of plasmonic particles, to date most of the work on plasmon- assisted reactions has been focused on the exploitation of co-catalytic effects related to hot-electron injection or charge separation, not for keeping the catalyst ‘clean’ or preventing its oxidation. The possibility of exploiting light as auxiliary tool for the control of the efﬁciency of a catalytic system has been investigated also at the macroscopic scale . This study has led to the development of a photo-actuated shutter that, according to the wavelength of the incident light, enables to regulate the activity of a photocatalyst deposed on the surface of the photoactuator, controlling the occurrence or the inhibition of a photochemical reaction. In this case, a mechanical system is utilized for the control of a classical photocatalytic system and light is exploited as parameter to modify microenvironment conditions of the catalytic system. Under UV illumination, the photoactuator is not active, it maintains a ﬂat conﬁguration and light can be exploited for making the desired photoreaction to occur. On the contrary, under visible illumination the photoactuator movement is activated, Catalysts 2021, 11, 64 7 of 18
protecting the chemical system from light and inhibiting the occurrence of the photochemi- cal reaction. The value of this approach has been demonstrated in the case of methylene blue photodegradation catalyzed by TiO2 nanoparticles, but the same principle could be exploited also in the case of different photoreactions.
2.4. Turning Problems into Opportunities: The Case of NiFe for Methane Dry Reforming and Chemical Looping
As discussed in the previous paragraph, CO2 can react with methane in a dry re- forming process to produce syngas, a mixture of hydrogen and carbon monoxide with a molar ratio around 1:1 (reaction 1). Among the variety of metals that have been screened to catalyze this reaction, Ni is one of the most investigated because of its low cost and high activity. In particular, Ni alloys have been extensively studied in view of their superior stability under operational conditions. Müller and co-workers demonstrated that NiFe alloys are able to generate a dynamic dealloying/re-alloying loop in response to changes of microenvironmental conditions during dry reforming, which prevents the formation of Catalysts 2021, 11, x FOR PEER REVIEW 8 of 19 carbon coke, improving the overall efﬁciency of the catalyst . The result is an adaptive catalyst, which is able to maintain its activity by dynamically modifying its phase (Figure3).
Figure 3. Example of self-regulating phase-change catalyst. See the main text and  for details. Figure 3. Example of self-regulating phase-change catalyst. See the main text and  for details. An important point to note is that Ni maintains its metallic state (Ni0) either in the An important point to note is that Ni maintains its metallic state (Ni0) either in the presence or absence of Fe. Thus, Fe is not active per se in dry reforming reaction, but plays presence or absencean indirect of Fe. Thus,key role, Fe iswhich not activecan be perunderstood se in dry by reforming considering reaction, the different but playscompetitive an indirect key role,reactio whichns occurring can be in understood dry reforming by considering the different competitive reactions occurring in dry reforming CH4 ⇄ 2 H2 + C (10)
CH4 2 HCO2 +2 C+ Fe ⇄ CO + FeO (10) (11) C + FeO ⇄ CO + Fe (12) CO2 + Fe CO + FeO (11) In NiFe alloys, during the interaction with CO2 Fe is partially oxidized to FeO (reac- C + FeO CO + Fe (12) tion 10), which induces partial dealloying of the catalyst. FeO forms few nm-thick small In NiFe alloys,domains during that the locate interaction preferentially with CO on2 Fe the is partiallycatalyst surface, oxidized protecting to FeO (reaction Ni from 10),coke for- which induces partialmation dealloying (reaction 9). ofAs the a result catalyst. of this FeO interaction forms fewwith nm-thickcarbon, FeO small is reduced domains back to Fe that locate preferentially(reaction on11), the which catalyst is reincorporated surface, protecting in Ni lattice Ni from (realloying). coke formation This beneficial (reaction Fe redox cycle avoids Ni deactivation and allows to sustain dry reforming. The best performances 9). As a result of this interaction with carbon, FeO is reduced back to Fe (reaction 11), were observed for a Ni4Fe composition. This is an example of active protection or catalyst which is reincorporated‘self-healing in Ni’. Unlike lattice the (realloying). case of plasmonic This beneﬁcial reduction, Fe which redox should cycle be avoids externally Ni acti- deactivation andvated allows by tolight sustain irradiation, dry reforming. in this case Thethe catalyst best performances directly exploits were coke observed formation, the for a Ni4Fe composition.major drawba Thisck is of an dry example reforming, of for active restoring protection the catalyst or catalyst to its initial ‘self-healing’. state. Unlike the case of plasmonicThis example reduction, introduces which two key should concepts be in externally design of systemic activated catalysts. by light irradiation, in this caseThe the first catalyst is related directly to the possibility exploits coke to turn formation, detrimental, the yet major unavoidable, drawback effects of into dry reforming, forpositive restoring (or even the es catalystsential) tofactors its initial to control state. the process course. This example introducesFor example, two D.Y. key Chung concepts et al. insuggested design ofto exploit systemic Cr(VI) catalysts. reduction to Cr(III) to ox- idize to CO2 the CO adsorbed on Pt catalyst, which usually causes inactivation of the cat- alysts in direct methanol fuel cells . This idea suggests an intriguing way to employ contaminated wastewater as an additive for the production of fuels (Figure 4).
Catalysts 2021, 11, x FOR PEER REVIEW 9 of 19
Catalysts 2021, 11, 64 8 of 18
The ﬁrst is related to the possibility to turn detrimental, yet unavoidable, effects into positive (or even essential) factors to control the process course. For example, D.Y. Chung et al. suggested to exploit Cr(VI) reduction to Cr(III) to oxidize to CO the CO adsorbed on Pt catalyst, which usually causes inactivation of the Catalysts 2021, 11, x FOR PEER REVIEW 2 9 of 19 catalysts in direct methanol fuel cells . This idea suggests an intriguing way to employ contaminated wastewater as an additive for the production of fuels (Figure4).
Figure 4. Scheme representing the use of toxic or unwanted reagents/byproducts to prevent catalyst’s deactivation. See  for details.
However, several critical issues remain still open, as in real water the concentration of a given pollutant cannot be sufficient to the scope and, in any case, it cannot be con- trolled a priori. In addition, the simultaneous presence of other interfering species with uncontrolled concentration makes the exploitation of the external chemical inputs a non- Figure 4. Scheme representingtrivial the task. use of toxic or unwanted reagents/byproducts to prevent catalyst’s deactivation. See  Figure 4. Scheme representing the use of toxic or unwanted reagents/byproducts to prevent catalyst’s deactivation. See for details.  for details. The second concept is chemical looping, which has been extensively investigated in the Müller’s group, for example in production of pure H2 or syngas from methane [44–46]. However, several critical issues remain still open, as in real water the concentration of The ideaHowever, at the basisseveral of critical chemical issues looping remain is still the open, generation as in real of watera sequence the concentration of chemical reac- a given pollutant cannot be sufﬁcient to the scope and, in any case, it cannot be controlled a of a given pollutant cannot be sufficient to the scope and, in any case, it cannot be con- tions,priori. aimed In addition, at obtaining the simultaneous a specific presence product of otherthat allows interfering to speciesuse and with regenerate uncontrolled a catalyst trolled a priori. In addition, the simultaneous presence of other interfering species with throughconcentration a circular makes process the exploitation originated of from the external concurrent chemical reactions inputs a(Figure non-trivial 2d). task. uncontrolled concentration makes the exploitation of the external chemical inputs a non- ForThe example, second concept as illustrated is chemical in looping,Figure 5 which, purehas H2 beencan be extensively obtained investigated from methane in the in three trivial task. stepsMüller’s that group, have forbeen example designed in production to utilize of and pure regenerate H or syngas a frommetalmethane oxide catalyst [44–46]. Thethrough a The second concept is chemical looping, which2 has been extensively investigated in redoxidea atcycle. the basis of chemical looping is the generation of a sequence of chemical reactions, theaimed Müller’s at obtaining group, afor speciﬁc example product in production that allows of topure use H and2 or regeneratesyngas from a catalyst methane through [44–46] a. In particular, methane is exploited to reduce the metal oxide, typically Fe2O3, (step 1) Thecircular idea process at the basis originated of chemical from concurrentlooping is the reactions generation (Figure of 2ad). sequence of chemical reac- totions, metallic aimed Fe, at which obtaining is in a specificturn partially product re that-oxidized allows toto use Fe 3andO4, byregenerate reacting a withcatalyst steam to For example, as illustrated in Figure5, pure H 2 can be obtained from methane in three generate highly pure H2 (step 2) and then fully oxidized in air to restore the Fe2O3 pristine throughsteps that a circular have been process designed originated to utilize from and conc regenerateurrent reactions a metal ( oxideFigure catalyst 2d). through a stateredox (stepFor cycle. example, 3). as illustrated in Figure 5, pure H2 can be obtained from methane in three steps that have been designed to utilize and regenerate a metal oxide catalyst through a redox cycle. In particular, methane is exploited to reduce the metal oxide, typically Fe2O3, (step 1) to metallic Fe, which is in turn partially re-oxidized to Fe3O4, by reacting with steam to generate highly pure H2 (step 2) and then fully oxidized in air to restore the Fe2O3 pristine state (step 3).
Figure 5. Example of chemical looping-based process for the production of H2 from CH4, using Figuremetal oxide5. Example as catalyst. of chemical See the mainlooping text- andbased [44 process,45] for details. for the production of H2 from CH4, using metal oxide as catalyst. See the main text and [44,45] for details.
In this loop, methane is combusted with molecular oxygen that is extracted from
Fe2O3 through a thermally-driven reduction. The metal oxide plays as the oxygen carrier, Figure 5. Example of chemical looping-based process for the production of H2 from CH4, using whichmetal oxideavoids as catalyst. the combustion See the main products text and [44,45] to mix for details.with either steam or H2. As a result, no additional steps of H2 separation and purification are required. This process is strongly In this loop, methane is combusted with molecular oxygen that is extracted from Fe2O3 through a thermally-driven reduction. The metal oxide plays as the oxygen carrier, which avoids the combustion products to mix with either steam or H2. As a result, no
additional steps of H2 separation and purification are required. This process is strongly
Catalysts 2021, 11, 64 9 of 18
In particular, methane is exploited to reduce the metal oxide, typically Fe2O3, (step 1) to metallic Fe, which is in turn partially re-oxidized to Fe3O4, by reacting with steam to generate highly pure H2 (step 2) and then fully oxidized in air to restore the Fe2O3 pristine state (step 3). In this loop, methane is combusted with molecular oxygen that is extracted from Fe2O3 through a thermally-driven reduction. The metal oxide plays as the oxygen carrier, which avoids the combustion products to mix with either steam or H2. As a result, no additional steps of H2 separation and puriﬁcation are required. This process is strongly dependent on the redox stability of iron oxide, which can be controlled by means of interactions with supporting substrates such as TiO2, Al2O3, MgAl2O4, and ZrO2. Müller and co-workers observed that the addition of Mn2O3 and ZrO2 to the Fe2O3 oxygen carrier improves the overall redox performances, allowing to achieve a stable production of highly pure H2. In particular, the formation of a Fe75Mn20Zr5 solid solution limits the high-temperature induced sintering and prevents the deposition of carbon coke that normally originates from methane cracking . In another example, the same group demonstrated that the addition of Cu to Ca2Fe2O5 oxygen carriers contributes to the stable production of pure H2 with high yields . At the origin of this improvement of performances there is the reversible exsolution/reincorporation of Cu nanoparticles. From a conceptual viewpoint, this behavior resembles the dealloying–alloying cycle discussed for NiFe catalyst. Here, Cu exsolution promotes methane oxidation, whereas its re-incorporation is essential to regenerate the pristine oxygen carrier. Reoxidation can be obtained by air exposure and it is a hallmark of Cu. Analogous experiments carried out with Ni in lieu of Cu revealed that exsolved Ni cannot by reincorporated into the Ca2Fe2O5 lattice, probably because Ni and Fe form NiFe alloys that tend to segregate separately. These studies highlight the importance of designing the components of a process through a careful evaluation of the structural dynamics occurring in the solid phase. In the case of syngas production, Donat and Müller demonstrated that a proper modiﬁcation 2+ of LaFeO3 perovskite oxygen carriers, obtained by a partial substitution of Sr (15%) in the La3+ sites and Al3+ (5%) in Fe3+ sites enables to promote a bulk phase transition that ∼ allows to transform methane and carbon dioxide in syngas with a H2/CO = 1 thorough chemical looping . Overall, chemical looping is a very interesting and universal approach, especially for high temperature reactions. In this regard, other remarkable examples applied to the ‘drop-in’ generation of syngas fuels directly from solar irradiation, have been reported by Steinfeld and co-workers . These studies demonstrated that a solar concentrator can be exploited to drive the endothermic reduction of the metal oxide catalyst, which is then reoxidized by reacting with steam and/or CO (Figure6). Among the large variety of MO/MO1-x metal oxide couples that have been tested, the CeO2-CeO2-x system was partic- ularly investigated, as it offers key advantages in terms of faster kinetics and improved stability and selectivity in comparison to other couples, such as those based on ferrites. Ceria was able to drive water and carbon dioxide splitting and produce syngas with a H2/CO ratio that can be easily controlled by tuning the amount of water and carbon diox- ide introduced in the reaction medium . The solar-to-fuel efﬁciency of these systems, which was quite limited (<1%) up to few years ago, has impressively grown in the last few years (around 5–6%) and it is expected to target the theoretical limit (20–30%) in the next future. In spite of still existing challenges, all strategies discussed in this paragraph represent an advancement of the concept of switching catalysts, which are becoming an emerging frontier also in heterogeneous catalysis . Catalysts 2021, 11, x FOR PEER REVIEW 11 of 19
CatalystsCatalysts 2021,2021 11, ,x11 FOR, 64 PEER REVIEW 10 of 1811 of 19
Figure 6. Example of chemical looping-based process for the production of syngas, using metal oxide (e.g., CeO2 or ZnO) as a catalyst. See the main text and [46,47] for details. Figure 6. Example of chemical looping-based process for the production of syngas, using metal oxide
Figure(e.g., CeO6. Example2 or ZnO) of as chemical a catalyst. looping See the-based main text process and [46 for,47 the] for production details. of syngas, using metal 2.5. Systemic Approaches for Oxygen Evolution Reaction (OER) oxide (e.g., CeO2 or ZnO) as a catalyst. See the main text and [46,47] for details. 2.5. Systemic Approaches for Oxygen Evolution Reaction (OER) Water splitting is a key process for the production of H2 from renewable sources. 2.5.However, SystemicWater splittingApproachesthe sluggish is afor key kinetics Oxygen process of Evolution foroxygen the production Reactionevolution (OER) ofreaction H2 from (OER) renewable is a major sources. bottleneck, However,which stro thengly sluggish impacts kinetics on the of performances oxygen evolution of reactionelectrochemical (OER) is aand major photoelectrochemical bottleneck, whichWater strongly splitting impacts is a on key the process performances for the of electrochemicalproduction of andH2 photoelectrochemicalfrom renewable sources. cells, as well as on the development of photocatalytic artificial leaves. OER is a four-elec- However,cells, as wellthe sluggish as on the kinetics development of oxygen of photocatalytic evolution reaction artiﬁcial (OER) leaves. is OERa major is a bottleneck, four- whichelectrontron stro reaction, reaction,ngly impacts which which usuallyon usually the performances implies aa sequence sequence of electrochemical of of multiple multiple reaction reactionand photoelectrochemical steps, steps, inﬂuenced influenced by cells,byformation formationas well asof of differenton different the development intermediate of species species photocatalytic [47 ]. . artificial leaves. OER is a four-elec- tron reaction,Thus,Thus, the thewhich catalysis catalysis usually of OERof OERimplies can can strongly a strongly sequence beneﬁt benefit of from multiple systemicfrom systemic reaction approaches. approaches.steps, In influenced a recent In a recent by formationpaper,paper, the the of Koper’s differentKoper’s group intermediategroup demonstrated demonstrated species that that alkali. alkali cations cations can be can a powerful be a powerful factor for factor for enhancingenhancingThus, the OER OER catalysis catalysed catalysed of byOER Ni-basedby can Ni- basedstrongly electrodes electrodes benefit , from as illustrated, systemicas illustrated in approaches. Figure in7 .Figure In 7 a. recent paper, the Koper’s group demonstrated that alkali cations can be a powerful factor for enhancing OER catalysed by Ni-based electrodes , as illustrated in Figure 7.
Figure 7. Example of manipulation of local microenvironment to improve OER. Enhancement of the activityFigure of7. aExample Ni-based of catalyst manipulation by alkali ions.of local See microenvironment the main text and [49 to] for improve details. OER. Enhancement of the activity of a Ni-based catalyst by alkali ions. See the main text and  for details. The catalytic activity of Ni electrodes is regulated by the formation of oxyhydroxide Figure 7. Example of manipulation of local microenvironment to improve OER. Enhancement of (NiOOH) species in the course of the process, which occurs in alkaline conditions at 1.4 V vs. the activityThe of catalytic a Ni-based activity catalyst of by Ni alkali electrodes ions. See is theregulated main text by and the  formation for details. of oxyhydroxide reversible(NiOOH) hydrogen species in electrode the course (RHE). of Previousthe process, works which by Boettcher occurs andin alkaline co-workers conditions pointed at 1.4 V out the role of Fe impurities in mediating the catalytic activity . The work of Koper’s vsThe. reversible catalytic hydrogen activity of electrode Ni electrodes (RHE). is regulatedPrevious byworks the formationby Boettcher of oxyhydroxideand co-workers andpointed co-workers out the shows role of that Fe alkali impurities ions have in amediating direct effect the in catalytic OER, even activity in the absence . The of work of (NiOOH)iron. In particular, species in the the combination course of the of in process, situ Raman which and occurs impedance in alkaline spectroscopy conditions enabled at 1.4 V Koper’s and co-workers shows that alkali ions have a direct effect in OER, even in the vsthe. reversible authors tohydrogen postulate electrode a new mechanism (RHE). atPrevious the basis works of the by enhanced Boettcher catalytic and effect,co-workers pointedwhichabsence reliesout of the iron. on role the In formationof particular, Fe impurities of the a superoxo combination in mediating NiOO —of Mthe in+ intermediatecatalyticsitu Raman activity and with imp differentedance. The M work +spectros- of Koper’salkalinecopy enabledand metals. co- workersthe These authors superoxo shows to postulate that species alkali area newions more mechanismhave stabilized a direct whenat theeffect larger basis in alkaliofOER, the metals evenenhanced in the cat- absencealytic ofeffect, iron. which In particular, relies on the the combination formation of of a superoxoin situ Raman NiOO and—M imp+ intermediateedance spectros- with dif- copyferent enabled M+ alkaline the authors metals. to postulateThese superoxo a new mechanismspecies are atmore the stabilizbasis ofed the when enhanced larger cat- alkali alyticmetals effect, (such which as Csrelies+) are on utilized the formation as the Mof +a source. superoxo Although NiOO— theM+ intermediatedetails of this with superoxo dif- - ferent M+ alkaline metals. These superoxo species are more stabilized when larger alkali metals (such as Cs+) are utilized as the M+ source. Although the details of this superoxo-
Catalysts 2021, 11, 64 11 of 18
(such as Cs+) are utilized as the M+ source. Although the details of this superoxo-assisted oxygen evolution are still under investigation, the effects on the overall OER processes are remarkable and clearly observed in both puriﬁed (i.e., iron-free) and non-puriﬁed electrolytic solutions. This example broadens the horizons of OER catalysis, which in the last years has been largely taking advantage of the dynamic modiﬁcations of the catalyst’s chemical composition [51–53], nanoalloying , and interactions with the substrate [55,56]. Another major goal in this ﬁeld is represented by water splitting from sea, or in general, saline waters. As mentioned before, the main issue in this regard is to keep OER separated from chlorine evolution (CER), which is not trivial as overpotential makes these two reactions concurrent in the potential range utilized to run water splitting. This competition originates from the different kinetics of the two processes. In particular, CER is a two-electron reaction that can be accomplished in a single catalytic step, which makes it faster than OER. Moreover, recent simulations revealed that OER and CER share the same catalytic centers. A way to tackle this competition was proposed in 2018 by Vos et al. and it is based on the deposition of a MnOx coating on the surface of IrOx catalysts, which are normally utilized to promote OER in acidic conditions . The MnOx layer prevents CER, yet allowing free in-and-out access for water, protons and oxygen to the IrOx catalytic centers. Strasser and co-workers recently utilized a systemic approach to solve the problem of OER vs. CER selectivity . The idea is based on water electrolyzers that utilized different electrolyte solutions to feed cathode and anode. In addition to the above-discussed competition between OER and CER as regards the potential range, the presence of chlorine ions in the water electrolyzer is detrimental for anion exchange membranes that are utilized to separate the cathodic and anodic compartment. The authors observed that NiFe-layered double hydroxide (NiFe-LDH) employed as catalyst for anodic OER exhibits optimized performances in alkaline environments, whereas saline water induces strong corrosion of both catalyst and porous transport layer. In order to circumvent this detrimental effect and allow NiFe-LDH catalysts to operate at their maximum efﬁciency, the electrolyzer was designed with a continuous feed of KOH solution at the anode, whereas the cathode is directly fed by seawater. This simple modiﬁcation of the system enabled the electrolyzer to operate with superior performances in comparison to analogous, yet symmetric, cells. Although many challenges remain to be addressed on the road towards seawater electrolysis, all the new strategies are expected to pass through a careful analysis of the overall system, including concurrent reactions and external factors that can be wisely exploited to assist the catalyst action. Moreover, photocatalytic water splitting, as well as direct generation of solar fuels, draws inspiration from photosynthesis. In this regard, a number of catalytic systems based on the Z-scheme approach have been designed and investigated in detail over the past years (Figure8). Here we observe that the Z-scheme, which is based on coupling between two photosystems connected by means of a common redox pathway, is a natural ﬁeld of application of system chemistry, with a large number of factors that can be controlled to maximize photon capture and reaction efﬁciency, such as the recent exploitation of multiphoton conversion and inorganic or hybrid optical nanoantennas [59–61]. The reader can refer to many excellent and updated reviews for a comprehensive overview [62,63]. Catalysts 2021, 11, x FOR PEER REVIEW 13 of 19
CatalystsCatalysts 20212021,, 1111,, x 64 FOR PEER REVIEW 1312 of of 19 18
Figure 8. Example of water splitting reactions based on the Z-scheme that couples two photosystems through a common Figure 8. Example of water splitting reactions based on the Z-scheme that couples two photosystems through a common redox cycle. A= Acceptor species; D= Donor species. See the main text and [62,63] for details. Figureredox cycle.8. Example A = Acceptor of water species; splitting D reactions = Donor species.based on See the the Z-scheme main text that and couples [62,63 ]two for details.photosystems through a common redox cycle. A= Acceptor species;2.6. Environmental D= Donor species. Remediation See the main text and [62,63] for details. 2.6. EnvironmentalEnvironmental Remediation remediation is another sector of catalysis in which a systemic ap- 2.6. Environmental Remediation proachEnvironmental can allow to remediationachieve major is another breakthroughs. sector of catalysisAlthough in most which of a the systemic literature approach is fo- cusedcan allowEnvironmental on the to achievecatalytic majorremediation degradation breakthroughs. is of another specific Although sectortargets, of most rea catalysisl systems of the literature in are which characterized is a focused systemic onby ap- the proachsimultaneouscatalytic can degradation allow presence to achieve of of speciﬁc many major targets,chemical breakthroughs. real species systems with Although are extremely characterized most variable of bythe the literatureconcentrations. simultaneous is fo- cusedpresenceMoreover, on the of the manycatalytic concentration chemical degradation species of these of with specific chemical extremely targets, species variable rea canl systems vary concentrations. not are only characterized from Moreover, one systemby the the simultaneoustoconcentration another, but presence of also these in theof chemical many same chemicalsystem species as canspecies a function vary with not ofextremely only time from under variable one the system mutual concentrations. to influence another, Moreover,ofbut different also in the the environmental concentration same system asfactorsof these a function (pH,chemical partialof time species pressure, under can the vary temperature, mutual not only inﬂuence from mass one of transport, different system toetcenvironmental another,.). This is but the also factors case, in for the (pH, example, same partial system pressure,of pollutants as a f temperature,unction dispersed of time mass in underwater transport, (rivers,the mutual etc.). sea, This influencelakes, is theaq- ofuifers,case, different for ground example, environmental-, waste of pollutants-, and factors tap dispersedwater), (pH, whose partial in water nature pressure, (rivers, and temperature,relative sea, lakes, concentration aquifers, mass transport, ground-, is typi- etcwaste-,cally.). Thisunpredictable and is tapthe water),case, a forpriori whose example, and nature largely of pollutants and influenced relative dispersed concentration by the abovein water- ismentioned typically (rivers, sea, unpredictablefactors. lakes, Anal- aq- uifers,ogous,a priori ground or and even largely- ,greater, waste inﬂuenced-, complexityand tap water), by is thecharacteristic whose above-mentioned nature of atmospheric and relative factors. pollutantsconcentration Analogous, and, oris in typi- evengen- callyeral,greater, unpredictableatmospheric complexity chem a is priori characteristicistry, and where largelyof meteorological atmospheric influenced by pollutants factors the above play and,- amentioned key in general, role in factors. determining atmospheric Anal- ogous,thechemistry, oscillations or even where greater, of meteorologicalrelative complexity concentration factors is characteristic playof gaseous a key of rolespecies. atmospheric in determining In view pollutants of finding the oscillations and, a practical in gen- of eral,applicationrelative atmospheric concentration in such chem complex ofistry, gaseous where and species.challenging meteorological In view environments, of factors ﬁnding play a practicala acatalyst key role application should in determining be inable such to thecopecomplex oscillations with and a variety challenging of relative of pollutants, environments,concentration interfering of a catalystgaseous species should species. and be dynamicIn able view to copeof modifications finding with aa varietypractical of the of applicationpollutants,external factors interferingin such (Figure complex species 9). and and challenging dynamic modiﬁcations environments, of the a catalyst external should factors be (Figure able 9to). cope with a variety of pollutants, interfering species and dynamic modifications of the external factors (Figure 9).
Figure 9. Scheme representing the main challenges of environmental remediation processes and the main features that Figure 9. Scheme representing the main challenges of environmental remediation processes and the main features that may enablemay enable the catalysts the catalysts to efﬁciently to efficiently remove remove toxic speciestoxic species or convert or convert them them into benign/value-added into benign/value-added products. products. Figure 9. Scheme representing the main challenges of environmental remediation processes and the main features that may enable the catalysts to efficientlyFor thisremove this reason, reason, toxic mostspecies most of ofor the theconvert catalysts catalysts them and into and strategies benign/value strategies tested- testedadded on products.onlab lab-scale-scale cannot cannot be ex- be tendedextended to real to real systems. systems. This gap This can gap be can bridged be bridged only by only shifting by shiftingthe paradigm the paradigm of catalyst’s of designcatalyst’sFor from this design reason,specificity from most speciﬁcity to of generality. the catalysts to generality. In otherand strategies words, In other researchers tested words, on researchers lab are-scale realizing cannot are realizing that be ex-the tendedquestthat the for to quest realoptimized systems. for optimized catalysts This gap catalysts specifically can be speciﬁcally bridged designed only designed forby shiftingthe degradation for thethe degradationparadigm of a given of ofcataly a target, givenst’s designtarget, shouldfrom specificity be accompanied to generality. with the In generation other words, of systemic researchers catalysts are realizing that can bethat active the questagainst for different optimized classes catalysts of compounds. specifically designed In a recent for paper, the degradation alginate-based of a activegiven target, blends
Catalysts 2021, 11, 64 13 of 18
have been employed as a coating layer for the most common ceramic photocatalysts (e.g., TiO2) and catalytic supports (Al2O3 and ZrO2) to adsorb cationic charged pollutants by means of a synergistic combination of electrostatic attraction and chemical afﬁnity . This concept of general decontaminant has been expanded in a recent paper focused on the development of photocatalysts for the degradation of different types of organic pollutants in water . These photocatalysts were rationally designed as modular systems, consisting of catalytic centers made of silver nanoparticles, which play the double role of catalysts and optical antennas, embedded into alginate hydrogel bubbles, which are utilized as dynamic sponges to adsorb polluted water. The silver nanoparticles are functionalized with β-Cyclodextrin, which are characterized by a general afﬁnity towards aryl- and heterocyclic ring-moieties. As most of the organic pollutants—such as dyes, biphenyls, and pharmaceutical compounds—contain these types of rings, these receptors act as universal scavengers for a large variety of pollutants. This pan-speciﬁc capture of organic pollutants represents an important advancement in comparison to previous works, which are often focused on the removal of individual compounds. Moreover, the presence of plasmonic silver nanoparticles allows not only the ultrasen- sitive detection of water pollutants by portable Raman spectrophotometers, but also their efﬁcient, light-driven degradation. In particular, two types of effects can be exploited: (a) the dynamic aggregation of the nanoparticles, induced by pollutant capture, which enables photo-assisted pollutant degradation or (b) pollutant light absorption capabilities. In this case the pollutant itself cooperates in its degradation. In the case of methylene blue, whose photosensitization produce singlet oxygen species, the pollutant can be utilized to destroy other pollutants, including bacteria or viruses, thus the overall catalyst is formed and evolves in the course of the process. Moreover, the pollutant capture-mediated aggregation of plasmonic nanoparticles is an efﬁcient way to exploit local plasmonic heating. This opto-thermal effect, which has been intensively investigated in the last years, represents a general way to induce the degradation of recalcitrant pollutants that do not absorb light in the visible. The plasmonic bubbles take advantage of this effect to efﬁciently remove antibiotics from water under direct sunlight irradiation, with obvious advantages for real world applications. In another recent work, Wei et al. applied plasmonic heating generated by silica-stabilized Janus gold nanorods to activate peroxydisulfate and promote oxidation of different classes of persistent organic pollutants under solar illumination . The degra- dation processes depend on the complex interplay among different phenomena, including photothermal heating, injection of hot-electrons and electron shuttling. In general, all reactions involving the formation of radical species can be approached from a systemic chemistry viewpoint. In 2019 Huang et al. demonstrated the possibility to induce decomplexation of Cu(II)-EDTA complexes and removal of Cu(II) species from real industrial wastewater by exploiting autocatalytic reactions triggered by UV irradiation of chlorine, which is usually utilized for water disinfection . Decomplexation is a key step in heavy metal recovery, as complexing agents effectively protect heavy metal ions from oxidation. In this regard, autocatalytic processes represent a major breakthrough for ad- vanced oxidation processes (AOP), which are normally based on UV/H2O2, UV/persulfate and photo-Fenton reactions and, in real systems, decrease their efﬁciency by interactions with other interfering species and/or due to pH variations . In the work of Huang , the production of highly efﬁcient Cl radicals is sustained by the continuous interconversion of Cu(I)/Cu(II) that proceeds through concurrent ligand- to-metal and metal-to-ligand charge transfer. As a result, Cu(II)-EDTA decomplexation follows an autocatalytic kinetics and the rapidly formed CuO precipitates and can be easily recovered without need of any further pH adjustment. Again, an appropriate exploitation of concurrent intermediates can overcome unsolved problems for traditional catalysis. All these approaches open the door to a variety of exciting applications for system chemistry. In the next future, the researchers could envision and design systemic cat- alysts through a synergistic combination of some of the concepts discussed above. In Catalysts 2021, 11, x FOR PEER REVIEW 15 of 19
easily recovered without need of any further pH adjustment. Again, an appropriate ex- ploitation of concurrent intermediates can overcome unsolved problems for traditional catalysis. Catalysts 2021, 11, 64 All these approaches open the door to a variety of exciting applications for system14 of 18 chemistry. In the next future, the researchers could envision and design systemic catalysts through a synergistic combination of some of the concepts discussed above. In particular, catalysts that are able to assist the degradation/conversion of wide classes of chemical particular, catalysts that are able to assist the degradation/conversion of wide classes of species, such as those containing an aromatic ring, which are characteristic of a large va- chemical species, such as those containing an aromatic ring, which are characteristic of riety of pharmaceutic compounds and many types of other organic pollutants, or fluori- a large variety of pharmaceutic compounds and many types of other organic pollutants, nated alkyl compounds, which encompass a few thousand different chemicals, could be or ﬂuorinated alkyl compounds, which encompass a few thousand different chemicals, rationally combined in catalytic cycles based on the synergistic interactions among exter- could be rationally combined in catalytic cycles based on the synergistic interactions among nal agents, reaction intermediates and byproducts (Figure 10). This kind of strategy could external agents, reaction intermediates and byproducts (Figure 10). This kind of strategy enablecould enable the simultaneous the simultaneous processing processing and and transformation transformation of of different different pollutan pollutantsts in in real world environments.
Figure 10. Scheme representing an example of systemic catalytic cycles based on synergistic interactions among different Figure 10. Scheme representing an example of systemic catalytic cycles based on synergistic interactions among different catalysts, reaction intermediates (Int 1, 2, ... , n) and byproducts and exploited for producing safe and value-added catalysts, reaction intermediates (Int 1, 2… n) and byproducts and exploited for producing safe and value-added com- compounds from environmental pollutants. pounds from environmental pollutants.
3. Conclusion Conclusionss and and Outlook This perspective brieflybrieﬂy discussed some recent examples of catalytic processes in complex sy systems,stems, focusing focusing the the attention attention on on approaches approaches and and strategies strategies that that are areable able to ex- to ploitexploit such such a complexity a complexity for forimproving improving catalytic catalytic performance. performance. In addition In addition to smart to smart cata- lysts,catalysts, which which are areable able to adapt to adapt and and respond respond toto external external stimuli, stimuli, the the rational rational manipulation manipulation anandd control of the local microenvironment is a key aspect in the design of any catalytic system operating in real world conditions. InIn particular, we observed that research in the ﬁeldfield of production of energy vectors fromfrom renewable sources can take full advantageadvantage of a detailed analysis of intermediate intermediate products and concurrentconcurrent reactions.reactions. InIn general,general, most most of of the the reactions reactions promoted promoted by by heteroge- hetero- genousnous catalysts catalysts are are severely severely affected affected by the by limited the limited lifetime lifetime of intermediates, of intermediates, which makes which makestheir spatial their spatial conﬁnement confinement and activation and activation into speciﬁc into specific reaction reaction pathways pathways crucial crucial factors fac- to torsachieve to achieve high turnover high turnover frequency frequency and selectivity. and selectivity. In this regard,In this regard, biology biology offers a offers rich palette a rich paletteof inspirational of inspirational examples, examples, such as such enzymes as enzymes and coupled and coupled reactions reactions involved involved in biological in bi- ologicalcycles and cycles photosynthesis and photosynthesis (Z-scheme). (Z-scheme). SignificantSigniﬁcant efforts efforts in in this this direction direction have have been been reported reported in recent in recent research research works, works, aimed aimedat triggering at triggering cascade cascade reactions reactions by means by ofmeans artiﬁcial of artificial enzymes enzymes (nanozymes) (nanozymes) or focused or fo- on cusedstabilizing on stabilizing intermediate intermediate species in species favorable in favorable conﬁgurations configurations and regulating and regulating the access the to accesscatalytic to activecatalytic sites. active Several sites. successful Several successful cases of application cases of application of chemical of chemical looping concepts looping to high-temperature reactions, such as syngas production or hydrogen puriﬁcation, have been reported in the last 2–3 years, and their number is expected to continuously grow in the near future. No matter the strategy applied for promoting the activation of small molecules (CO2, H O, CH , CO, NH , etc.) utilized to generate energy vectors, solar fuels or value-added 2 4 3 products, in the research community there is an ever-increasing attention to ﬁnd solutions that go beyond the static approaches that have been normally utilized so far. Catalysts 2021, 11, 64 15 of 18
A particularly interesting feature of systemic strategies is that, in some cases, detri- mental factors, such as the formation of byproducts or the presence of contaminants, can be turned into useful, or even key, ingredients for improving the efﬁciency of the overall catalytic process. This kind of symbiosis could become a new paradigm in the design of catalysts, also for environmental remediation, which is an inherently complex ﬁeld. The examples discussed from this perspective also note the importance of achiev- ing detailed information about all the factors and reaction pathways that can occur in a given process and their mutual interactions. In the case of complex systems, this could be a formidable task to accomplish. However, the giant leaps forward in development of machine learning and artiﬁcial intelligence-based algorithms can represent a powerful tool for catalyst’s design. At present, these algorithms are intensively utilized for screen- ing among a variety of possible combinations of materials and compositions, in order to ﬁnd optimal solutions for heterogeneous catalysis . These analyses mainly rely on thermodynamic data and DFT simulations. However, the synergistic integration of these algorithms with experimental data obtained from in-situ and operando-like characteriza- tion techniques [70,71] could lead to the design of groundbreaking, alternative catalytic systems that are able to harness complexity to ﬁnd out-of-the box solutions to compelling problems, especially in the ﬁelds of energy vectors and environmental remediation .
Author Contributions: Conceptualization, I.A. and I.V.; Writing—original draft preparation, I.A. and I.V.; Writing—review and editing, I.A. and I.V.; Visualization, I.A. and I.V.; Supervision, I.A. and I.V. All authors have read and agreed to the published version of the manuscript. Funding: This research was partially funded by EU and Regione Lombardia, “POR-FESR 2014- 2020/Innovazione e Competitività”, in the framework of the project: BioMass HUB. Conﬂicts of Interest: The authors declare no conﬂict of interest. The funders had no role in the design of the study; in the collection, analyses, or interpretation of data; in the writing of the manuscript, or in the decision to publish the results.
References 1. Ludlow, R.F.; Otto, S. Systems chemistry. Chem. Soc. Rev. 2008, 37, 101–108. [CrossRef][PubMed] 2. Ashkenasy, G.; Hermans, T.M.; Otto, S.; Taylor, A.F. Systems chemistry. Chem. Soc. Rev. 2017, 46, 2543–2554. [CrossRef] 3. Semenov, S.N.; Kraft, L.J.; Ainla, A.; Zhao, M.; Baghbanzadeh, M.; Campbell, V.E.; Kang, K.; Fox, J.M.; Whitesides, G.M. Autocat- alytic, bistable, oscillatory networks of biologically relevant organic reactions. Nature 2016, 537, 656–660. [CrossRef][PubMed] 4. Bissette, A.J.; Fletcher, S.P. Mechanisms of autocatalysis. Angew. Chem. Int. Ed. 2013, 52, 12800–12826. [CrossRef][PubMed] 5. Blackmond, D.G. An Examination of the Role of Autocatalytic Cycles in the Chemistry of Proposed Primordial Reactions. Angew. Chem. 2009, 121, 392–396. [CrossRef] 6. Yoshida, R.; Murase, Y. Self-oscillating surface of gel for autonomous mass transport. Colloids Surf. B Biointerfaces 2012, 99, 60–66. [CrossRef][PubMed] 7. Tabata, O.; Hirasawa, H.; Aoki, S.; Yoshida, R.; Kokufuta, E. Ciliary motion actuator using self-oscillating gel. Sens. Actuators A Phys. 2002, 95, 234–238. [CrossRef] 8. Maeda, S.; Hara, Y.; Sakai, T.; Yoshida, R.; Hashimoto, S. Self-walking gel. Adv. Mater. 2007, 19, 3480–3484. [CrossRef] 9. Chen, I.C.; Kuksenok, O.; Yashin, V.V.; Balazs, A.C.; Van Vliet, K.J. Mechanical resuscitation of chemical oscillations in Belousov- Zhabotinsky gels. Adv. Funct. Mater. 2012, 22, 2535–2541. [CrossRef] 10. Vassalini, I.; Alessandri, I. Spatial and Temporal Control of Information Storage in Cellulose by Chemically Activated Oscillations. ACS Appl. Mater. Interfaces 2015, 7, 28708–28713. [CrossRef] 11. Yang, T.H.; Zhou, S.; Gilroy, K.D.; Figueroa-Cosme, L.; Lee, Y.H.; Wu, J.M.; Xia, Y. Autocatalytic surface reduction and its role in controlling seed-mediated growth of colloidal metal nanocrystals. Proc. Natl. Acad. Sci. USA 2017, 114, 13619–13624. [CrossRef][PubMed] 12. Maity, I.; Dev, D.; Basu, K.; Wagner, N.; Ashkenasy, G. Signaling in Systems Chemistry: Programing Gold Nanoparticles Formation and Assembly Using a Dynamic Bistable Network. Angew. Chem. Int. Ed. 2020, 59, 1–7. [CrossRef] 13. Twilton, J.; Le, C.C.; Zhang, P.; Shaw, M.H.; Evans, R.W.; MacMillan, D.W.C. The merger of transition metal and photocatalysis. Nat. Rev. Chem. 2017, 1.[CrossRef] 14. Allen, A.E.; MacMillan, D.W.C. Synergistic catalysis: A powerful synthetic strategy for new reaction development. Chem. Sci. 2012, 3, 633–658. [CrossRef][PubMed] 15. Chen, R.; Neri, S.; Prins, L.J. Enhanced catalytic activity under non-equilibrium conditions. Nat. Nanotechnol. 2020, 15, 868–874. [CrossRef] Catalysts 2021, 11, 64 16 of 18
16. Lubrano Lavadera, M.; Song, Y.; Sabia, P.; Herbinet, O.; Pelucchi, M.; Stagni, A.; Faravelli, T.; Battin-Leclerc, F.; De Joannon, M. Os- cillatory Behavior in Methane Combustion: Inﬂuence of the Operating Parameters. Energy Fuels 2018, 32, 10088–10099. [CrossRef] 17. Tiemersma, T.P.; Kolkman, T.; Kuipers, J.A.M.; van Sint Annaland, M. A novel autothermal reactor concept for thermal coupling of the exothermic oxidative coupling and endothermic steam reforming of methane. Chem. Eng. J. 2012, 203, 223–230. [CrossRef] 18. Rofer-DePoorter, C.K. A Comprehensive Mechanism for the Fischer-Tropsch Synthesis. Chem. Rev. 1981, 81, 447–474. [CrossRef] 19. Catlow, C.R.A.; Wells, P.; Gianolio, D. Synchrotron radiation techniques in catalytic science. Phys. Chem. Chem. Phys. 2020, 22, 18745–18746. [CrossRef] 20. Alessandri, I. Enhancing raman scattering without plasmons: Unprecedented sensitivity achieved by TiO2 shell-based resonators. J. Am. Chem. Soc. 2013, 135, 5541–5544. [CrossRef] 21. Alessandri, I.; Vassalini, I.; Bertuzzi, M.; Bontempi, N.; Memo, M.; Gianoncelli, A. “RaMassays”: Synergistic Enhancement of Plasmon-Free Raman Scattering and Mass Spectrometry for Multimodal Analysis of Small Molecules. Sci. Rep. 2016, 6, 1–8. [CrossRef][PubMed] 22. Alessandri, I.; Carletti, L.; Ferroni, M.; De Angelis, C.; Vassalini, I. Bioinspired self-similar all-dielectric antennas: Probing the effect of secondary scattering centres by Raman spectroscopy. Mater. Adv. 2020, 1, 2443–2449. [CrossRef] 23. Bontempi, N.; Vassalini, I.; Alessandri, I. All-dielectric core/shell resonators: From plasmon-free SERS to multimodal analysis. J. Raman Spectrosc. 2018, 49, 943–953. [CrossRef] 24. Bontempi, N.; Vassalini, I.; Danesi, S.; Alessandri, I. ZORRO: Zirconium oxide resonators for all-in-one Raman and whispering- gallery-mode optical sensing. Chem. Commun. 2017, 53, 10382–10385. [CrossRef][PubMed] 25. Vassalini, I.; Rotunno, E.; Lazzarini, L.; Alessandri, I. “stainless” Gold Nanorods: Preserving Shape, Optical Properties, and SERS Activity in Oxidative Environment. ACS Appl. Mater. Interfaces 2015, 7, 18794–18802. [CrossRef][PubMed] 26. Bontempi, N.; Vassalini, I.; Danesi, S.; Ferroni, M.; Donarelli, M.; Colombi, P.; Alessandri, I. Non-Plasmonic SERS with Silicon: Is It Really Safe? New Insights into the Optothermal Properties of Core/Shell Microbeads. J. Phys. Chem. Lett. 2018, 9, 2127–2132. [CrossRef] 27. DeRita, L.; Resasco, J.; Dai, S.; Boubnov, A.; Thang, H.V.; Hoffman, A.S.; Ro, I.; Graham, G.W.; Bare, S.R.; Pacchioni, G.; et al. Structural evolution of atomically dispersed Pt catalysts dictates reactivity. Nat. Mater. 2019, 18, 746–751. [CrossRef][PubMed] 28. Alessandri, I.; Bañares, M.A.; Depero, L.E.; Ferroni, M.; Fornasiero, P.; Gennari, F.C.; Hickey, N.; Martinez-Huerta, M.V.; Montini, T. Structural investigation of Ce2Zr2O8 after redox treatments which lead to low temperature reduction. Top. Catal. 2006, 41, 35–42. [CrossRef] 29. Vassalini, I.; Alessandri, I. Switchable stimuli-responsive heterogeneous catalysis. Catalysts 2018, 8, 569. [CrossRef] 30. Moussallem, I.; Jörissen, J.; Kunz, U.; Pinnow, S.; Turek, T. Chlor-alkali electrolysis with oxygen depolarized cathodes: History, present status and future prospects. J. Appl. Electrochem. 2008, 38, 1177–1194. [CrossRef] 31. Zhu, S.; Wang, D. Photocatalysis: Basic principles, diverse forms of implementations and emerging scientiﬁc opportunities. Adv. Energy Mater. 2017, 7, 1–24. [CrossRef] 32. Wang, X.; Xu, A.; Li, F.; Hung, S.F.; Nam, D.H.; Gabardo, C.M.; Wang, Z.; Xu, Y.; Ozden, A.; Rasouli, A.S.; et al. Efﬁcient Methane Electrosynthesis Enabled by Tuning Local CO2 Availability. J. Am. Chem. Soc. 2020, 142, 3525–3531. [CrossRef][PubMed] 33. Li, F.; Thevenon, A.; Rosas-Hernández, A.; Wang, Z.; Li, Y.; Gabardo, C.M.; Ozden, A.; Dinh, C.T.; Li, J.; Wang, Y.; et al. Molecular tuning of CO2-to-ethylene conversion. Nature 2020, 577, 509–513. [CrossRef][PubMed] 34. O’Mara, P.B.; Wilde, P.; Benedetti, T.M.; Andronescu, C.; Cheong, S.; Gooding, J.J.; Tilley, R.D.; Schuhmann, W. Cascade Reactions in Nanozymes: Spatially Separated Active Sites inside Ag-Core-Porous-Cu-Shell Nanoparticles for Multistep Carbon Dioxide Reduction to Higher Organic Molecules. J. Am. Chem. Soc. 2019, 141, 14093–14097. [CrossRef][PubMed] 35. Yang, P.P.; Zhang, X.L.; Gao, F.Y.; Zheng, Y.R.; Niu, Z.Z.; Yu, X.; Liu, R.; Wu, Z.Z.; Qin, S.; Chi, L.P.; et al. Protecting Copper Oxidation State via Intermediate Conﬁnement for Selective CO2 Electroreduction to C2+ Fuels. J. Am. Chem. Soc. 2020, 142, 6400–6408. [CrossRef] 36. Jeon, H.S.; Timosnenko, J.; Scholten, F.; Sinev, I.; Herzog, A.; Haase, F.T.; Cuenya, B.R. Operando insight into the correlation between the structure and composition of CuZn nanoparticles and their selectivity for the electrochemical CO2 reduction. J. Am. Chem. Soc. 2020, 141, 19879–19887. [CrossRef] 37. Albinsson, D.; Boje, A.; Nilsson, S.; Tiburski, C.; Hellman, A.; Ström, H.; Langhammer, C. Copper catalysis at operando conditions—bridging the gap between single nanoparticle probing and catalyst-bed-averaging. Nat. Commun. 2020, 11, 1–13. [CrossRef] 38. Zhong, Y.; Xu, Y.; Ma, J.; Wang, C.; Sheng, S.; Cheng, C.; Li, M.; Han, L.; Zhou, L.; Cai, Z.; et al. An Artiﬁcial Electrode/Electrolyte Interface for CO2 Electroreduction by Cation Surfactant Self-Assembly. Angew. Chem. Int. Ed. 2020, 132, 19257–19263. [CrossRef] 39. Kim, D.; Kley, C.S.; Li, Y.; Yang, P. Copper nanoparticle ensembles for selective electroreduction of CO2 to C2–C3 products. Proc. Natl. Acad. Sci. USA 2017, 114, 10560–10565. [CrossRef] 40. Marimuthu, A.; Zhang, J.; Linic, S. Tuning Selectivity in Propylene Epoxidation by Plasmon Mediated Photo-Switching of Cu Oxidation State. Science 2013, 339, 1590–1593. [CrossRef] 41. Vassalini, I.; Alessandri, I. “The phactalysts”: Carbon nanotube/TiO2 composites as phototropic actuators for wireless remote triggering of chemical reactions and catalysis. Nanoscale 2017, 9, 11446–11451. [CrossRef][PubMed] Catalysts 2021, 11, 64 17 of 18
42. Kim, S.M.; Abdala, P.M.; Margossian, T.; Hosseini, D.; Foppa, L.; Armutlulu, A.; Van Beek, W.; Comas-Vives, A.; Copéret, C.; Müller, C. Cooperativity and dynamics increase the performance of NiFe dry reforming catalysts. J. Am. Chem. Soc. 2017, 139, 1937–1949. [CrossRef] 43. Chung, D.Y.; Kim, H.; Chung, Y.H.; Lee, M.J.; Yoo, S.J.; Bokare, A.D.; Choi, W.; Sung, Y.E. Inhibition of CO poisoning on Pt catalyst coupled with the reduction of toxic hexavalent chromium in a dual-functional fuel cell. Sci. Rep. 2014, 4, 1–5. [CrossRef][PubMed] 44. Hosseini, D.; Donat, F.; Abdala, P.M.; Kim, S.M.; Kierzkowska, A.M.; Müller, C.R. Reversible Exsolution of Dopant Im- proves the Performance of Ca2Fe2O5 for Chemical Looping Hydrogen Production. ACS Appl. Mater. Interfaces 2019, 11, 18276–18284. [CrossRef] 45. Hosseini, D.; Donat, F.; Kim, S.M.; Bernard, L.; Kierzkowska, A.M.; Müller, C.R. Redox-Driven Restructuring of FeMnZr- Oxygen Carriers Enhances the Purity and Yield of H2 in a Chemical Looping Process. ACS Appl. Energy Mater. 2018, 1, 1294–1303. [CrossRef] 46. Donat, F.; Müller, C.R. CO2-free conversion of CH4 to syngas using chemical looping. Appl. Catal. B Environ. 2020, 278.[CrossRef] 47. Marxer, D.; Furler, P.; Takacs, M.; Steinfeld, A. Solar thermochemical splitting of CO2 into separate streams of CO and O2 with high selectivity, stability, conversion, and efﬁciency. Energy Environ. Sci. 2017, 10, 1142–1149. [CrossRef] 48. Romero, M.; Steinfeld, A. Concentrating solar thermal power and thermochemical fuels. Energy Environ. Sci. 2012, 5, 9234–9245. [CrossRef] 49. Garcia, A.C.; Touzalin, T.; Nieuwland, C.; Perini, N.; Koper, M.T.M. Enhancement of Oxygen Evolution Activity of Nickel Oxyhydroxide by Electrolyte Alkali Cations. Angew. Chem. Int. Ed. 2019, 58, 12999–13003. [CrossRef] 50. Trotochaud, L.; Young, S.L.; Ranney, J.K.; Boettcher, S.W. Nickel-Iron oxyhydroxide oxygen-evolution electrocatalysts: The role of intentional and incidental iron incorporation. J. Am. Chem. Soc. 2014, 136, 6744–6753. [CrossRef] 51. Gorlin, Y.; Chung, C.J.; Benck, J.D.; Nordlund, D.; Seitz, L.; Weng, T.C.; Sokaras, D.; Clemens, B.M.; Jaramillo, T.F. Understanding interactions between manganese oxide and gold that lead to enhanced activity for electrocatalytic water oxidation. J. Am. Chem. Soc. 2014, 136, 4920–4926. [CrossRef] 52. Gorlin, M.; De Araujo, J.F.; Schmies, H.; Bernsmeier, D.; Dresp, S.; Gliech, M.; Jusys, Z.; Chernev, P.; Kraehnert, R.; Dau, H.; et al. Tracking catalyst redox states and reaction dynamics in ni-fe oxyhydroxide oxygen evolution reaction electrocatalysts: The role of catalyst support and electrolyte pH. J. Am. Chem. Soc. 2017, 139, 2070–2082. [CrossRef][PubMed] 53. Frydendal, R.; Busch, M.; Halck, N.B.; Paoli, E.A.; Krtil, P.; Chorkendorff, I.; Rossmeisl, J. Enhancing activity for the oxygen evolu- tion reaction: The beneﬁcial interaction of gold with manganese and cobalt oxides. ChemCatChem 2015, 7, 149–154. [CrossRef] 54. Vassalini, I.; Borgese, L.; Mariz, M.; Polizzi, S.; Aquilanti, G.; Ghigna, P.; Sartorel, A.; Amendola, V.; Alessandri, I. Enhanced Electrocatalytic Oxygen Evolution in Au–Fe Nanoalloys. Angew. Chem. Int. Ed. 2017, 56, 6589–6593. [CrossRef][PubMed] 55. Zou, S.; Burke, M.S.; Kast, M.G.; Fan, J.; Danilovic, N.; Boettcher, S.W. Fe (Oxy)hydroxide Oxygen Evolution Reaction Elec- trocatalysis: Intrinsic Activity and the Roles of Electrical Conductivity, Substrate, and Dissolution. Chem. Mater. 2015, 27, 8011–8020. [CrossRef] 56. Yeo, B.S.; Bell, A.T. Enhanced activity of gold-supported cobalt oxide for the electrochemical evolution of oxygen. J. Am. Chem. Soc. 2011, 133, 5587–5593. [CrossRef] 57. Vos, J.G.; Wezendonk, T.A.; Jeremiasse, A.W.; Koper, M.T.M. MnOx/IrOx as Selective Oxygen Evolution Electrocatalyst in Acidic Chloride Solution. J. Am. Chem. Soc. 2018, 140, 10270–10281. [CrossRef] 58. Dresp, S.; Ngo Thanh, T.; Klingenhof, M.; Brückner, S.; Hauke, P.; Strasser, P. Efﬁcient direct seawater electrolysers using selective alkaline NiFe-LDH as OER catalyst in asymmetric electrolyte feeds. Energy Environ. Sci. 2020, 13, 1725–1729. [CrossRef] 59. Salmistraro, M.; Schwartzberg, A.; Bao, W.; Depero, L.E.; Weber-Bargioni, A.; Cabrini, S.; Alessandri, I. Triggering and monitoring plasmon-enhanced reactions by optical nanoantennas coupled to photocatalytic beads. Small 2013, 9, 3301–3307. [CrossRef] 60. Salmistraro, M.; Sassolini, S.; Weber-Bargioni, A.; Cabrini, S.; Alessandri, I. Fabrication of gold nanoantennas on SiO2/TiO2 core/shell beads to study photon-driven surface reactions. Microelectron. Eng. 2015, 143, 69–73. [CrossRef] 61. Ravetz, B.D.; Pun, A.B.; Churchill, E.M.; Congreve, D.N.; Rovis, T.; Campos, L.M. Photoredox catalysis using infrared light via triplet fusion upconversion. Nature 2019, 565, 343–346. [CrossRef][PubMed] 62. Proppe, A.H.; Li, Y.C.; Aspuru-Guzik, A.; Berlinguette, C.P.; Chang, C.J.; Cogdell, R.; Doyle, A.G.; Flick, J.; Gabor, N.M.; van Grondelle, R.; et al. Bioinspiration in light harvesting and catalysis. Nat. Rev. Mater. 2020, 5, 828–846. [CrossRef] 63. Ng, B.J.; Putri, L.K.; Kong, X.Y.; Teh, Y.W.; Pasbakhsh, P.; Chai, S.P. Z-Scheme Photocatalytic Systems for Solar Water Splitting. Adv. Sci. 2020, 7.[CrossRef][PubMed] 64. Vassalini, I.; Gjipalaj, J.; Crespi, S.; Gianoncelli, A.; Mella, M.; Ferroni, M.; Alessandri, I. Alginate-Derived Active Blend Enhances Adsorption and Photocatalytic Removal of Organic Pollutants in Water. Adv. Sustain. Syst. 2020, 4, 1–11. [CrossRef] 65. Vassalini, I.; Ribaudo, G.; Gianoncelli, A.; Casula, M.F.; Alessandri, I. Plasmonic hydrogels for capture, detection and removal of organic pollutants. Environ. Sci. Nano 2020.[CrossRef] 66. Wei, H.; Loeb, S.K.; Halas, N.J.; Kim, J.-H.; David Waite, T.; Wang, J. Plasmon-enabled degradation of organic micropollutants in water by visible-light illumination of Janus gold nanorods. Proc. Natl. Acad. Sci. USA 2020, 27, 15473–15481. [CrossRef] 67. Huang, X.; Wang, Y.; Li, X.; Guan, D.; Li, Y.; Zheng, X.; Zhao, M.; Shan, C.; Pan, B. Autocatalytic Decomplexation of Cu(II)-EDTA and Simultaneous Removal of Aqueous Cu(II) by UV/Chlorine. Environ. Sci. Technol. 2019, 53, 2036–2044. [CrossRef] 68. Cuerda-Correa, E.M.; Alexandre-Franco, M.F.; Fern, C. Antibiotics from Water. An Overview. Water 2020, 12, 102. [CrossRef] Catalysts 2021, 11, 64 18 of 18
69. Schlexer Lamoureux, P.; Winther, K.T.; Garrido Torres, J.A.; Streibel, V.; Zhao, M.; Bajdich, M.; Abild-Pedersen, F.; Bligaard, T. Machine Learning for Computational Heterogeneous Catalysis. ChemCatChem 2019, 11, 3581–3601. [CrossRef] 70. Enman, L.J.; Stevens, M.B.; Dahan, M.H.; Nellist, M.R.; Toroker, M.C.; Boettcher, S.W. Operando X-ray Absorption Spectroscopy Shows Iron Oxidation is Concurrent with Oxygen Evolution in Cobalt–Iron (Oxy)hydroxide Electrocatalysts. Angew. Chem. Int. Ed. 2018, 57, 12840–12844. [CrossRef] 71. Dou, J.; Sun, Z.; Opalade, A.A.; Wang, N.; Fu, W.; Tao, F. Operando chemistry of catalyst surfaces during catalysis. Chem. Soc. Rev. 2017, 46, 2001–2027. [CrossRef][PubMed] 72. Centi, G.; Cejka, J. Needs and Gaps for Catalysis in Addressing Transitions in Chemistry and Energy from a Sustainability Perspective. ChemSusChem 2019, 12, 621–632. [CrossRef][PubMed]